Polishing process in naval industry:
improvement of an existing
electro-mechanical polishing machine
Treball Final de Grau
Facultat de Nàutica de Barcelona
Universitat Politècnica de Catalunya
Treball realitzat per:
Jordi Perramon Terricabras
Jordi Torralbo Gavilán
Xavier Martínez García
Grau en Enginyeria en Sistemes i Tecnologia Naval
Barcelona, Octubre 2018
First of all, I would like to give my gratitude’s to my final project tutor’s; Jordi Torralbo Gavilán and Xavier Martínez García. Thanks for all the support and help during all this long time since I have started.
I would like to mention all the staff of Hispana de Maquinaria S.A. that have helped me and have given all the facilities during this process. Also, for the opportunity of taking part of the all the polishing projects that they have started more than 10 years ago.
En aquest estudi pretenc estudiar tots aquells elements de llautó i bronze del món naval els quals requereixen d’excel·lents acabats superficials. Normalment, per aconseguir aquest acabat es requereix un procediment de polit, el qual es fa amb maquinaria especialitzada.
El projecte està dividit principalment en dues parts. En la primera enumeraré algunes de les solucions existents que s’utilitzen en les industries per l’acabat de les superfícies. Explicaré el procés, la màquina, els consumibles que s’utilitzen i donaré també algunes pautes pel desbastat i polit del llautó i bronze. La segona part del projecte estarà enfocada en un dels processos en particular; el polit electro-mecànic. Descriuré la màquina, que actualment s’utilitza únicament en el món de la joieria. A més a més, enumeraré tots els seus punts dèbils; trencament d’alguna part degut a la fatiga, corrosió d’algunes parts degut al compost, esquitxades de compost degut el moviment del raspall, etc.
Finalment, donaré algunes propostes de millora en totes aquestes parts (a fi de millorar l’eficiència, el funcionament, el manteniment i la qualitat), per tal de que continuï sent una màquina competitiva en el mercat de les màquines de polit.
This study aims to be an analysis of the different brass and bronze naval elements which require excellent surfaces. To get this finish, all those parts needs a polishing process made with a machine.
The project will be divided in two main parts. In the first one I will list some of the different existing processes used in industries for finishing pieces surfaces. I will explain the process, the machine, the consumables used and I will also give some parameters used for grinding and polishing brass and bronze. The second part of the project will be focused in one particular process; electro-mechanical polishing. I will describe the machine, nowadays used only for jewellery, and all the failures existing; break of some parts of the machine due to fatigue, corrosion of some electrical parts due to the compound, splashes of compound due to the movement of the sliding brush, etc.
Afterwards, I will give some ideas in order to upgrade all these parts of the machine and improve it (the efficiency, operation, maintenance and quality), for continue being competitive in the market of polishing machines.
Table of contents
TABLE OF CONTENTS VII
FIGURES LIST X
TABLES LIST XIII
GRAPHICS LIST XIV
CHAPTER 1. INTRODUCTION. 1
CHAPTER 2. BRASS AND BRONZE. 5
2.1.1 BRIEF HISTORY OF BRASS 5
2.1.2 BRASS DESCRIPTION 6
2.2.1 BRIEF HISTORY OF BRONZE 10
2.2.2 BRONZE DESCRIPTION 11
2.3MAIN DIFFERENCES BETWEEN USING BRASS AND BRONZE 13 2.4USES OF BRASS AND BRONZE IN NAVAL INDUSTRY 14
CHAPTER 3. POLISHING METHODS. 19
3.2MANUAL POLISHING 21
3.2.1. THEORY OF THE SYSTEM 21
3.2.2. DESCRIPTION OF THE MACHINE 22
3.2.3. MATERIALS USED FOR POLISHING 24
ABRASIVE WHEELS 24
POLISHING PASTES 29
3.2.4. PARAMETERS RECOMMENDED FOR POLISHING BRASS AND BRONZE 32
3.2.5. ADVANTAGES AND DISADVANTAGES OF THE SYSTEM 33
3.3DISC FINISHING MACHINE 35
3.3.1. THEORY OF THE SYSTEM 35
3.3.2. DESCRIPTION OF THE MACHINE 36
3.3.3. MATERIALS USED FOR POLISHING 38
3.3.5. ADVANTAGES AND DISADVANTAGES OF THE SYSTEM 43
3.4VIBRATORY POLISHING MACHINE 45
3.4.1. THEORY OF THE SYSTEM 45
3.4.2. DESCRIPTION OF THE MACHINE 46
3.4.3. MATERIALS USED FOR POLISHING 48
3.4.4. PARAMETERS RECOMMENDED FOR POLISHING BRASS AND BRONZE 54
3.4.5. ADVANTAGES AND DISADVANTAGES OF THE SYSTEM 54
3.5BARREL FINISHING MACHINE 56
3.5.1. THEORY OF THE SYSTEM 56
3.5.2. DESCRIPTION OF THE MACHINE 57
3.5.3. MATERIALS USED FOR POLISHING 60
3.5.4. PARAMETERS RECOMMENDED FOR POLISHING BRASS AND BRONZE 61
3.5.5. ADVANTAGES AND DISADVANTAGES OF THE SYSTEM 61
3.6ELECTRO-POLISHING MACHINE 63
3.6.1. THEORY OF THE SYSTEM 63
3.6.2. DESCRIPTION OF THE MACHINE 65
3.6.3. MATERIALS USED FOR POLISHING 68
3.6.4. PARAMETERS RECOMMENDED FOR POLISHING BRASS AND BRONZE 69
3.6.5. ADVANTAGES AND DISADVANTAGES OF THE SYSTEM 70
CHAPTER 4. ELECTRO-MECHANICAL POLISHING. 72
4.1.THEORY OF THE SYSTEM 72 4.2.DESCRIPTION OF THE MACHINE 74 4.3.MATERIALS USED FOR POLISHING 83 4.4.PARAMETERS RECOMMENDED FOR POLISHING BRASS AND BRONZE 84
4.5.ADVANTAGES AND DISADVANTAGES OF THE SYSTEM 85
CHAPTER 5. PROBLEMS IN THE EN-34. 87
5.1.ELECTRICAL ISOLATION OF THE CONNECTIONS 87
5.1.1 ANODE CONNECTIONS 87
5.1.2 CATHODE CONNECTION 88
5.2.MECHANICAL RESIZING 89
5.2.1. SLIDING BRUSH 89
5.2.2. NEW MOTOR 89
5.3.SPLASHING OF THE COMPOUND 90 5.4.PRESSURE SPRING FOR RACK 93
5.5.RINSING TANK 94
5.6.JUNCTION BETWEEN WORKING TANK AND ELECTRICAL CABINET PLATE SEPARATOR 94
6.1.ELECTRICAL ISOLATION OF THE CONNECTIONS 97
6.1.1. ANODE CONNECTIONS 97
6.1.2. CATHODE CONNECTION 99
6.2.MECHANICAL RESIZING 101
6.2.1. SLIDING BRUSH 101
6.2.2. NEW MOTOR 105
6.3.SPLASHING OF THE COMPOUND 106
6.3.1. INCREASE THE WORKING TANK HEIGHT 106
6.3.2. CHANGES IN THE METALLIC STRUCTURE 107
6.3.3. AVOID SPLASHES INSIDE THE ELECTRONIC CABINET 108
6.4.PRESSURE SPRING FOR RACK 108
6.5.RINSING TANK 109
6.6.JUNCTION BETWEEN WORKING TANK AND ELECTRICAL CABINET PLATE SEPARATOR 109
CHAPTER 7. DISCUSSIONS AND CONCLUSIONS 111
FIGURE 1. EN-34 MACHINE ... 2
CHAPTER 2.BRASS AND BONZE FIGURE 2. BRASS PROFILES ... 5
FIGURE 3. CRYSTAL STRUCTURE OF BRASS DEPENDING ON TEMPERATURE (ºC) – ZINC CONTENT (%) ... 7
FIGURE 4. PIECES MADE WITH NAVAL BRASS. ... 9
FIGURE 5. BRONZE PROFILES ... 10
FIGURE 6. FIRST WEAPONS MADE OF BRONZE ... 11
FIGURE 7. NAVAL PROPELLER MADE OF BRASS ... 11
FIGURE 8. BRONZE HINGE ... 14
FIGURE 9. BRONZE LOCK ... 14
FIGURE 10. BRASS HANDLE ... 15
FIGURE 11. BRONZE WALL LAMP ... 15
FIGURE 12. BRONZE ANTIQUE CLOCK ... 15
FIGURE 13. BRONZE THROUGH-HULL... 16
FIGURE 14. BRONZE VALVE... 16
FIGURE 15. BRONZE TRUNK CONNECTION ... 16
FIGURE 16. SMALL BRONZE PROPELLER ... 17
FIGURE 17. BRONZE PROPELLERS ... 17
CHAPTER 3.POLISHING METHODS FIGURE 18. REFLECTION DIFFERENCES IN A POLISHED / NOT POLISHED SURFACE ... 19
FIGURE 19. USE OF A MANUAL POLISHING MOTOR ... 22
FIGURE 20. BENCH GRINDER ... 22
FIGURE 21. PEDESTAL GRINDER ... 23
FIGURE 22. GRINDER USED MAINLY IN JEWELLERY ... 23
FIGURE 23. DIFFERENTIATE PARTS OF A BENCH GRINDER ... 24
FIGURE 24. DIFFERENT EXAMPLES OF ABRASIVE WHEELS ... 25
FIGURE 25. DIFFERENT COTTON POLISHING WHEELS ... 26
FIGURE 26. DIFFERENT SIZES OF FELT WHEELS ... 26
FIGURE 27. STEEL WIRE WHEEL ... 27
FIGURE 28. NYLON WHEEL ... 27
FIGURE 29. ALUMINIUM OXIDE WHEEL ... 28
FIGURE 30. SILICON CARBIDE WHEEL ... 28
FIGURE 31. DIFFERENT EXAMPLES OF POLISHING PASTES ... 29
FIGURE 32. BLACK COMPOUND FOR MANUAL POLISHING... 30
FIGURE 33. BROWN COMPOUND FOR MANUAL POLISHING ... 30
FIGURE 34. WHITE ROUGE COMPOUND FOR MANUAL POLISHING ... 31
FIGURE 35. RED ROUGE COMPOUND FOR MANUAL POLISHING ... 31
FIGURE 37. TAN COMPOUND FOR MANUAL POLISHING ... 32
FIGURE 38. ORANGE-GLOW COMPOUND FOR MANUAL POLISHING ... 32
FIGURE 39. BLUE MAGIC COMPOUND FOR MANUAL POLISHING ... 32
FIGURE 40. POLISHING A BRONZE PROPELLER INSIDE THE WATER WITH AN ANGULAR GRINDING MACHINE ... 34
FIGURE 41. MOVEMENT OF THE PIECES INSIDE THE DISC FINISHING MACHINE ... 35
FIGURE 42. DISC FINISHING MACHINE WITH TWO DRUMS: FOR DRY AND WET POLISHING ... 36
FIGURE 43. PARTS OF THE DISC FINISHING MACHINE ... 37
FIGURE 44. CONTROL PANEL OF A DISC FINISHING MACHINE ... 38
FIGURE 45. SIEVE USED TO SEPARATE MEDIA FROM PIECES... 38
FIGURE 46. DIFFERENT MEDIA TYPES ... 39
FIGURE 47. PLASTIC GRINDING CHIPS FOR WET DISC FINISHING ... 39
FIGURE 48. CERAMIC ABRASIVE MEDIA FOR WET DISC FINISHING ... 40
FIGURE 49. WALNUT SHELL MEDIA FOR DRY DISC POLISHING ... 41
FIGURE 50. DRY GRINDING GRANULATES FOR DRY DISC POLISHING ... 41
FIGURE 51. PLASTIC POLISHING CHIPS FOR DRY DISC POLISHING ... 42
FIGURE 52. CORN GRANULATES FOR DRY DISC POLISHING ... 42
FIGURE 53. POLISHING PASTE AND GRINDING OIL FOR DRY DISC POLISHING ... 42
FIGURE 54. UNLOADING THE MEDIA AND THE PIECES FROM THE MACHINE... 43
FIGURE 55. MOVEMENT OF THE PIECES INSIDE THE VIBRATORY MACHINE ... 45
FIGURE 56. EXAMPLE OF A VIBRATORY MACHINE OF HIGH CAPACITY ... 46
FIGURE 57. MIX OF PIECES AND MEDIA INSIDE A VIBRATORY MACHINE ... 46
FIGURE 58. MAIN PARTS OF THE VIBRATORY MACHINE ... 47
FIGURE 59. VIBRATORY MACHINE WITH THE SYSTEM FLOW-THROUGH, WHICH AUTOMATICALLY SEPARATES MEDIA AND PIECES ... 48
FIGURE 60. DIFFERENT SHAPES FOR STEEL MEDIA ... 50
FIGURE 61. DIFFERENT SHAPES FOR CERAMIC MEDIA ... 51
FIGURE 62. DIFFERENT SHAPES FOR PLASTIC MEDIA ... 52
FIGURE 63. EXAMPLES OF DIFFERENT SHAPES AND SIZES OF HARDWOOD MEDIA ... 53
FIGURE 64. CORN COB GRIT MEDIA ... 53
FIGURE 65. WALNUT SHELL MEDIA ... 54
FIGURE 66. MIX OF WATER, MEDIA AND PIECES INSIDE A BARREL ... 56
FIGURE 67. EXAMPLE OF A BARREL FINISHING MACHINE ... 58
FIGURE 68. HEXAGONAL BARREL ... 59
FIGURE 69. DIFFERENT SHAPES FOR PLASTIC MEDIA ... 60
FIGURE 70. ELECTRO-POLISHING MACHINE WITH A RINSING TANK ... 63
FIGURE 71. APPARITION OF THE VISCOUS LAYER OVER THE METAL ... 64
FIGURE 72. RELATION BETWEEN THE VOLTAGE AND THE CURRENT DENSITY... 64
FIGURE 73. MAINS PARTS OF THE ELECTRO-POLISHING MACHINE ... 66
FIGURE 74. ELECTRO-POLISHING TANK WITH CATHODES PLACED INSIDE THE BATH ... 67
FIGURE 75. ANODIC RACK INSIDE THE TANK ... 68
CHAPTER 4.ELECTRO-MECHANICAL POLISHING FIGURE 76. GOLD RING BEFORE/AFTER BEING POLISHED WITH THE ELECTRO-MECHANICAL POLISHING MACHINE ... 72
FIGURE 77. THE ACTION OF THE SMALL PARTICLES OVER ALL THE PIECE SURFACE ... 72
FIGURE 78. GENERAL VIEW OF THE EN-34 ... 73
FIGURE 79. ANODIC RACK WITH HOOKS, WHERE THE PIECES ARE HANGED ... 74
FIGURE 80. GENERAL VIEW OF INSIDE THE WORKING TANK ... 75
FIGURE 81. INTERIOR OF THE ELECTRICAL CABINET (1) ... 76
FIGURE 82. INTERIOR OF THE ELECTRICAL CABINET (2) ... 76
FIGURE 83. ELECTRICAL CABINET PLATE SEPARATOR ... 76
FIGURE 84. PARTS 1 AND 2 ARE THE METALLIC COVER OF THE EN-34... 77
FIGURE 85. PROGRAMMING PANEL OF THE MACHINE ... 78
FIGURE 86. VIEW OF AN EMPTY WORKING TANK ... 79
FIGURE 87. ANODIC CONNECTION TO THE RACK, FITTED INSIDE THE WORKING TANK ... 79
FIGURE 88. STAINLESS STEEL CATHODE ... 80
FIGURE 89. ORGANIC CATHODE ... 80
FIGURE 90. SLIDING BRUSH FOR EN-34... 81
FIGURE 91. FIX BRUSH FOR EN-34 ... 81
FIGURE 92. DRIVING HEAD FITTED ON THE ELECTRICAL CABINET PLATE SEPARATOR, WITH THE BRUSH AT ITS END ... 82
FIGURE 93. RINSING TANK FITTED IN FRONT OF THE EN-34 ... 83
FIGURE 94. MIXED COMPOUND ENSI010 INSIDE THE CAN, BEFORE POURING IT TO THE MACHINE ... 84
FIGURE 95. SILVER RING BEFORE/AFTER BEING POLISHED WITH THE ELECTRO-MECHANICAL POLISHING MACHINE ... 85
CHAPTER 5.PROBLEMS IN THE EN-34 FIGURE 96. VIEW OF THE ANODIC CONNECTION INSIDE THE WORKING TANK ... 87
FIGURE 97. WIRES PLACED OUTSIDE THE WORKING TANK FOR THE ANODIC AND CATHODIC CONNECTIONS ... 88
FIGURE 98. CONNECTION INSIDE THE WORKING TANK BETWEEN THE CATHODE AND THE NEGATIVE WIRE... 88
FIGURE 99. APPROACHING OF THE SLIDING BRUSH TO THE FIX BRUSH ... 91
FIGURE 100. APPROACHING OF THE SLIDING BRUSH TO THE WORKING TANK ... 91
FIGURE 101. METALLIC PLATE WHICH COVERS THE WORKING TANK ... 92
FIGURE 102. SPLASHING PLASTIC PROTECTORS, FITTED OVER THE METALLIC PLATE ... 92
FIGURE 103. ALL THE PROTECTIONS AGAINST THE SPLASHING FITTED IN THE MACHINE ... 93
FIGURE 104. PRESSURE SPRING FOR THE RACK ... 93
FIGURE 105. EARS THAT HOLDS THE TANK TO THE MACHINE ... 94
FIGURE 106. JUNCTION USED BETWEEN THE WORKING TANK AND THE ELECTRICAL CABINET PLATE SEPARATOR, WHICH PREVENTS WALL BENDING ... 95
CHAPTER 6.SUGGESTIONS FOR IMPROVING THE EN-34 FIGURE 107. CONNECTION FOR THE ANODIC WIRE ... 98
FIGURE 108. THE FEMALE TERMINAL PROPOSED ... 98
FIGURE 109. THE MALE TERMINAL PROPOSED ... 98
FIGURE 110. A PLATING MACHINE, WITH CATHODIC BARS ... 99
FIGURE 111. SCHEMATIC DRAWING OF THE NEW CATHODE CONNECTION... 100
FIGURE 112. BROKEN SLIDING BRUSH DUE TO FATIGUE ... 101
FIGURE 113. GRAPHIC OF S-N FOR AISI316 ... 103
TABLE 1. GOLD PROPERTIES ... 3
TABLE 2. SILVER PROPERTIES ... 4
CHAPTER 2.BRASS AND BRONZE TABLE 3. MAIN BRASS ALLOYS ... 8
TABLE 4. MAIN PROPERTIES OF MOST USED BRASSES ... 9
TABLE 5. MAIN BRONZE ALLOYS ... 12
TABLE 6. MAIN PROPERTIES OF MOST USED BRONZES ... 12
TABLE 7. MAIN DIFFERENCES BETWEEN USING BRASS AND BRONZE... 13
CHAPTER 3.POLISHING METHODS TABLE 8. PUNCTUATION FOR MANUAL POLISHING ... 34
TABLE 9. PUNCTUATION FOR DISC FINISHING ... 44
TABLE 10. PUNCTUATION FOR VIBRATORY FINISHING ... 56
TABLE 11. PUNCTUATION FOR BARREL FINISHING ... 62
TABLE 12. PARAMETERS TO POLISH BRASS AND BRONZE IN ELECTRO-POLISHING MACHINE (1) ... 69
TABLE 13. PARAMETERS TO POLISH BRASS AND BRONZE IN ELECTRO-POLISHING MACHINE (2) ... 70
TABLE 14. PUNCTUATION FOR ELECTRO-POLISHING FINISHING ... 71
CHAPTER 4.ELECTRO-MECHANICAL POLISHING TABLE 15. PUNCTUATION FOR ELECTRO-MECHANICAL FINISHING ... 86
CHAPTER 5.PROBLEMS IN THE EN-34 TABLE 16. CHARACTERISTICS OF THE ACTUAL MOTOR INSTALLED IN THE EN-34 ... 90
CHAPTER 6.SUGGESTIONS FOR IMPROVING THE EN-34 TABLE 17. NEW MOTOR CHOSEN FOR THE EN-34 ... 105
CHAPTER 7.DISCUSSIONS AND CONCLUSIONS TABLE 18. COMPARISON OF ALL POLISHING METHODS DESCRIBED ... 112
GRAPHIC 1. METALS POLISHED WITH THE EN-34 ... 2
CHAPTER 3.POLISHING METHODS GRAPHIC 2. MAIN POLISHING SOLUTIONS ... 21
GRAPHIC 3. ABRASIVES WHEELS USED FOR MANUAL POLISHING ... 25
GRAPHIC 4. COMPOUNDS USED FOR MANUAL POLISHING ... 30
GRAPHIC 5. MATERIAL USED FOR WET POLISHING IN DISC FINISHING MACHINES ... 39
GRAPHIC 6. MATERIAL USED FOR DRY POLISHING IN DISC FINISHING MACHINES ... 41
Chapter 1. Introduction.
There are some industries where great quality finishing surfaces are demanded. This causes that during years new machines have been developed in order to have best results possible for grinding and polishing pieces. In the following text, I will talk about the different industrial polishing methods used for finishing pieces; starting from manual polishing, through rotatory machines with abrasive inside and electro-polishing, until new methods developed during this last decade for a Spanish company seated in Barcelona; Hispana de Maquinaria S.A.
For almost three years ago I started working with this company which developed an innovative system for grinding and polishing jewellery, called electro-mechanical polishing. Due to most jewellery pieces needs perfect surfaces, a new system with better performances is necessary for this industry.
EN-34, machine developed for electro-mechanical polishing, can process different alloys depending on the compound used. All the compounds are formed by liquid (oils and chemicals) and resins, which allows the pass of current.
Inside the working tank, where the compound is poured, there are an anode and a pair of cathodes. The anode (+) is connected to the rack where the pieces are hanged. The cathode (-) is a metallic plate where the metal is adhered during the process. Thanks to the pass of current between the anode and the cathode, starts the electro-polishing of the pieces hanged on the rack.
The metal adhered at the cathode can be recovered, for example, by burning the cathode. This is very important for the jewellery industry, where precious metals are used. Silver, but especially gold, are very expensive materials, so by recovering them the customer can recover money.
Inside the working tank there are also a pair of brushes, one of them moved by a motor. The purpose of these brushes is touching the surface of the pieces hanged in the rack with their hair, allowing the pass of current. They are also used to push the resins of the compound inside all the interior parts. Thanks to this continuous mechanical movement of the brushes it is possible to process the pieces.
This machine, which has to be placed on top of a table, has a total dimensions of 450 x 390 x 370 mm. Its weight is approximately of 32 Kg, and with the compound reaches 40 Kg. The consumption of the machine is 400W.
Figure 1. EN-34 machine. Source: Own
In the following lines I will describe the main metal alloys that can be grinded and polished with the EN-34 machine. The compound is made specifically for each metal, so good results are achieved in more pure alloys, in those ones which there is less content of other metals.
Graphic 1. Metals polished with the EN-34. Source: Own
It is the most popular metal used in jewellery. The electro-mechanical polishing machine EN-34, can polish all kind of gold alloys with the same compound (only by changing the parameter). It is possible to classify this metal depending on:
- Karats GRINDING AND POLISHING GOLD WHITE GOLD YELLOW GOLD RED GOLD SILVER COPPER ALLOYS BRASS BRONZE
3 Gold is a soft chemical element when it is pure (24K), so it is usually alloyed with other metals, typically used for jewellery. Those additions increase its hardness, ductility, melting point and colour, as well as many other properties.
The addition of those other metals reduces the gold percentage, which means that the gold has less karats. Most typical combinations are 24K, 22K, 18K, 14K or 10K.
As told before, with the addition of other metals it is possible to change the properties of the gold. One of the properties is the colour, so depending on the metal alloyed with the gold, it is possible to classify it by colours:
• Yellow gold
It is an alloy of gold, and usually similar percentages of copper and silver (10-15% of each one). Due to the high content of gold, the yellow colour is maintained.
• White gold
It is an alloy of gold and nickel, manganese or palladium. Those three metals give the white colour to the alloy.
• Red gold
It is an alloy of gold and high content of copper. Thanks to the high content of copper, the alloy gets reddish.
In the following table I will describe the main properties of 24K gold:
GOLD Density (g/cm3) Melting point (ºC) Tensile Strength (MPa) Yield Strength (MPa) Elongation (%) Thermal conductivity (W/m·ºK) Electrical conductivity (S/m) Hardness (Rockwell B) 19.32 1064.43 120 205 30 318 4.1·107 25
Table 1. Gold properties. Source: www.matweb.com
Silver is also one of the most popular metals in jewellery. Fine silver (or also called pure silver, which is 99,9% silver) is very soft. To increase the hardness and strength is necessary to add some other metals. The most popular silver is Sterling silver, which has 92,5% of silver and the rest 7,5% by weight is composed by other alloys (usually copper).
Even though there are other silver compositions, with the EN-34 machine it is only possible to get good polishing results with Sterling silver.
4 SILVER Density (g/cm3) Melting point (ºC) Tensile Strength (MPa) Yield Strength (MPa) Elongation (%) Thermal conductivity (W/m·ºK) Electrical conductivity (S/m) Hardness (Rockwell B) 10.491 961.93 140 54 25 419 6.3·107 30
Table 2. Silver properties. Source: www.matweb.com
c) Copper alloys
In jewellery, and mainly in costume jewellery, are used cheaper metals based in copper. After all the proceeding, a plating is made in the piece surface (normally with gold). Those alloys are:
- Brass. Obtained basically by mixing copper and zinc. - Bronze. Obtained basically by mixing copper and tin.
Both metals can be polished with the EN-34, obtaining good results in surface finishing and shinning of the piece.
Of all those metals described before, brass and bronze are not only used for jewellery, they are also used in naval industry. Propellers and decorative parts of the ship are made of these alloys, as good as plumbing accessories. Those metals are recommended due to their good strength properties and high corrosion resistance, in comparison with other metals with approximately the same price.
In conclusion, it is possible to process those metal pieces for naval purposes with the EN-34, moving away from the traditional machines.
This machine has entered in the market before being tested carefully. This not enough checking of the machine, causes a lot of problems in customers factory. This factor added to the sharp competition with other companies of the sector, which have copied the electro-mechanical polishing process, force us to improve the machine in order to get the best machine of the market.
As I am working in the technical department, I am directly in touch with the customers so I know which are the main problems that they face during production. Knowing these problems of the EN-34, the main goal of this project is do all the possible changes in order to get a more efficient and without so many fails. All those changes have to be done under the following premises:
- Improve the performance of the machine after hours of working.
- Do not change some working parameters stablished in order to not change the quality of the surface.
- Maintain the producing cost of the EN-34, in order to do not increase the sale price.
- In order to improve the maintenance of the machine, it is important to make an easier removal of the working tank.
Chapter 2. Brass and bronze.
Brass is the most used copper alloy and it is obtained basically by mixing copper and zinc. Depending on the proportions of each material and the mixing temperature, the final metal has different properties. The mechanical and physical chemistry properties of the brass will change depending on the metals range used, and also on the metals added to the alloy.
Figure 2. Brass profiles. Source: www.copper.org
2.1.1 Brief history of brass
After the “Copper Age” comes the “Bronze Age”, followed later by the “Iron Age”. The reason is very simple; there was not “Brass age” because of the difficulty of getting zinc before the 18th century. Despite this fact, people get brass from using ground smithsonite ore (calamine, ZnCO3) and mixing it in high temperatures with copper. We know that this metal was used:
- Roman people used a brass called “Aurichalum” in order to have sesterces coins and golden coloured helmets. The contain of zinc was about 11 – 28% and it is only added for decorative and ornamental purposes. For ornament pieces, which needs a more ductile metal, they usually use 18% of zinc.
- In Medieval ages, brass was mainly used in churches and monuments. The content of zinc was between 23-29%, and they give small additions of lead and tin to the alloy.
With the Industrial Revolution the brass became more important, so an easiest way to get the zinc was needed. In 1738, William Champion take out the patent of zinc production by distillation from calamine and charcoal.
Thanks to the invention of Muntz 60/40 brass, was possible to reduce the prices of hot workable brass plates. For example, this allows the use of brass instead of copper for the sheathing of wooden ships (preventing biofouling and worm attack).
In 1894, Alexander Dick revolutionize the production of good quality and low-cost rods, by inventing a new extrusion press. Subsequent developments in the production have improved the final product, as good as reduced the price of brass.
2.1.2 Brass description
Brass is a very common material for equipment’s in all industries. Due to the combination of its properties, it is a very valuable material for wide uses. For example:
- Its machinability is better than in many other materials.
- It can be easily casted to get de desired shape. It is also good to fabricate pieces by extrusion, rolling, hot stamping and cold forming.
- It can usually be used without any protection layer.
- Brass is usually chosen for producing low cost machined products.
Brass is mainly done by mixing cooper and zinc. The percentage of zinc and the temperature can change the atomic crystal structure, so it is possible to divide it in different categories depending on their crystal structure. Basically, three types of brass structures can be differentiated depending on the content ratio of materials and the temperature of mixing.
a) Alpha brasses (>65% of Copper)
They crystalize in the cubic system centered on the faces. Those type of metals are also called cold working brasses due to they are the only kind of brasses malleable and worked at cold.
Basically, their main characteristics are their high ductility at room temperature, so they can be deformed by rolling, drawing, shearing, bending of the plate, stretching the metal, spinning and thread rolling.
b) Beta brasses (50-55% of Copper)
This metal crystallizes at the cubic system centered in the body (BCC). Above the critical temperatures (approximately 500ºC) the zinc atoms start moving randomly. When the temperature decrease, each atom moves to their preferential position. In conclusion, in phase beta and under the critical temperature, the zinc atoms stay in its preferential position, causing very large organized grids.
c) Alpha – beta brasses (55-65% of Copper).
It is a combination of both brasses above. That type of metal does not allow the deformation at room temperature due to the content of beta phase, in other words this brass works better with higher temperatures. This allows to the brass to be extruded into bars or tubes, and hot forged in matrices.
7 By decreasing the Beta phase and increasing Alpha (by being more an alpha structure), it is possible to obtain very good properties in machinability and easy to deform in lower temperatures.
Figure 3. Crystal structure of brass depending on Temperature (ºC) – Zinc content (%). Source: www.cimsaww.com
As told before, the addition of different metals to the alloy can also change the properties. The following alloys are the most common used:
Proportion by weight (%)
Other metals Characteristics Copper Zinc Tin Lead
90 10 - - -
69 30 1 - - Tin doesn’t allow the loss of zinc in many environments.
Aich’s alloy 60.60 36.58 1.08 - 1.74% Iron Used in marine service due its hardness and toughness, also as for its good performance against corrosion.
77.5 20.5 - - 2% Aluminum Aluminium improves corrosion resistance.
Common brass or Rivet brass
63 37 - - - Standard for cold working and it is also very cheap.
Delta metal 55 41-43 - - 1-3% Iron The addition of iron makes a harder material.
Free machining brass
61.5 35.15 - 3 0.35 Iron Good machinability.
Gilding metal 95 5 - - - Softest brass available. High brass 65 35 - - - High tensile strength. Low brass 80 20 - - - Very ductile.. Manganese
70 28.7 - - 1.3% Manganese
Muntz metal 60 40 - - Traces of Iron
Naval brass 59 40 1 - - Similar to admiralty brass. Nickel brass 70 24.5 - - 5.5% Nickel
Nordic gold 89 5 1 - 5% Aluminium Prince’s metal 75 25 - - -
Red brass 85 5 5 5 -
Silicon tombac 80 16 - - 4% Silicon
Tombac 95-80 5-20 - - - Cheap and hand malleable alloy Yellow brass 67 33 - - -
Table 3. Main brass alloys. Source: www.thoughtco.com
In conclusion, as it is possible to see in the table before, there are many kinds of brasses depending on the alloy added. Each alloy will change some main properties of the brass.
Depending on the zinc addition, the colour of the brass can change from red to yellow. Thanks to this property, brasses are used for decorative applications.
If copper content is higher than 63%, the brass is very malleable at room temperature. When copper content is lower than 63%, and there are no other kind of metals alloyed, the ductility decreases, so these metals have to been worked with heat.
All brasses have good machining properties, but the addition of lead improves this property (makes softer brasses).
9 - Corrosion resistance
Brasses has good properties against corrosion, but for marine environments is recommended to add some tin to the alloy.
- Dezincification resistance
Brasses with more than 15% of zinc need little additions of arsenic to improve the dezincification. - Wear resistance
Normally, adding silicon or tin to the alloy improves the wear resistance of the brass.
In the next table it is possible to see the differences in properties between most used brasses in industry.
Brass alloy Density (g/cm3) Melting point (ºC) Tensile Strength (MPa) Yield Strength (MPa) Elongation (%) Thermal conductivity (W/m·ºK) Electrical conductivity (S/m) Hardness (Rockwell B) Red Brass 8.75 988 393 338 12 159.2 2.2·107 56 Cartridge brass 8.53 916 427 359 25 121.2 1.6·107 54 Muntz Metal 8.39 899 483 345 10 122.9 1.6·107 85 Naval Brass 8.41 888 483 400 17 116.0 1.5·107 25
Table 4. Main properties of most used brasses. Source: www.copper.org
Brass is usually used in naval industry due to its great mechanical properties, and also due to the high corrosion resistance. It is mainly used for propeller shafts, marine hardware, decorative fittings and turn buckles. In conclusion, most used brasses for naval industry are:
• Aich’s alloy
• Admiralty brass
• Naval brass
In chapter 2.4 I will give more information about the use of brass in naval industry, giving some examples of pieces made of this metal.
Common bronze is an alloy obtained basically from mixing copper and tin, and depending on the proportions of each material, the final metal has different properties. Tin is usually alloyed in proportions from 0.5% to 11% of the total weight, depending on the properties desired of the final metal.
It is also possible to add some other metals for upgrading the alloy. For example, phosphor, aluminium, manganese and silicon are usually added to bronze in order to increase its properties.
Figure 5. Bronze profiles. Source: www.bronmetal.com
2.2.1 Brief history of bronze
The first apparition of copper alloyed with tin is in Pločnik, Serbia. There is an ace head which is dated approximately in 4500 BC, before the “Bronze Age”. This new material allows to replace the stone, getting more possibilities in terms of shapes (thanks to the casting). The apparition of this metal improves the manufacture of weapons and tools.
The use of bronze mainly starts with the “Bronze Age”. It is difficult to date it because depending the region started in different centuries. It is possible to divide the “Bronze Age” in the following periods:
- Around 3000 BC, brass is commonly used to manufacture weapons, ornaments and fitting for chariots. One of the firsts dated brass objects dated, is a knife found in China, which has been casted in a mould. Most of the bronzes are alloyed also with arsenic, which led to poisoning. Due to this, bronze was used during several years (although tin was more difficult to obtain).
- By 2500 BC, tin is the most favourite metal alloyed with bronze. Casting techniques have been improved, so it is possible to create human sized statues.
- During 2000 BC, the use of bronze started being more common in Egypt and China. Firsts years, these two civilizations used sand for bronze casting, basically to create objects like bells. Eventually, they improve the technique and start using moulds made from clay and stone.
11 Figure 6. First weapons made of bronze. Source: www.monaghan.ie
After this age, in 800 BC, the bronze was very used in ship constructions due to its properties against oxidation in comparison with iron alloys. Bronze creates a superficial oxidation layer of copper oxide, which forms a protective barrier.
Despite the gunpowder was discovered in China around 800AD (used to create the first firearms), this technology arrives at Europe in the 13th century. Brass was mainly used due to the small metal friction for firing iron cannon bullets.
Nowadays, bronze has a lot of applications in our life. For example:
- Aluminium bronze is quite hard and is usually used for springs, bearings and car gearbox bearings. - As bronze does not make sparks when it hits against other surfaces, is an ideal material for
hammers, mallets or any other tool used in flammable environment.
- Phosphor bronze is usually used for ships propellers thanks to the good properties of this material against rusting.
- Most of the musical instruments are made of bronze. Most cymbals and bells are made of this material.
2.2.2 Bronze description
As told before, common bronze is composed basically from copper and tin (from 0.5 to 11%). Depending on the proportions of each material, the final metal has different properties. It is possible to divide bronze in different categories, depending on the addition of other metals to the main alloy.
The following alloys are the most common used:
Proportion by weight
(%) Other metals Characteristics
Phosphor bronze 89 – 99 0.5 - 11 0.01 – 0.35% phosphor High strength and durability. High fatigue resistance and low friction coefficient. Good properties against corrosion. Aluminium bronze 89 - 95 - 5 – 11 % aluminium
Other alloys in small quantities
Higher tensile strength and resistance than other bronze alloys. Good performance against wear and heavy loads.
The apparition of the alumina prevents the metal of being corroded. This makes the material resistant to sea water, also preventing the accumulation of sea life and marine organisms.
Manganese bronze 66 - 75 1 2.5 – 5 % manganese 22 – 28 % zinc
Ideal for high loads due to its high strength properties and hardness.
Silicon bronze 95 – 97.5 - 2.5 – 5 % silicon
Zinc, manganese or tin in small quantities
Hard material with high strength in different temperatures.
Good properties against corrosion.
Table 5. Main bronze alloys. Source: www.zoresrecycling.com
In the next table it is possible to see the differences in properties between most used brasses in industry.
Bronze alloy Density (g/cm3) Melting point (ºC) Tensile Strength (MPa) Yield Strength (MPa) Elongation (%) Thermal conductivity (W/m·ºK) Electrical conductivity (S/m) Hardness (Rockwell B) Aluminium bronze 7.45 1040 586 221 12 58.6 0.7·107 92 Silicon bronze 8.53 971 676 363 8 36.3 0.41·107 40 Phosphor bronze 8.86 954 517 448 25 69.2 0.9·107 26
13 Bronze is usually used in naval industry due to its great mechanical properties and also due to the high corrosion resistance. It is mainly used for propeller shafts, marine hardware, decorative fittings and turn buckles. In conclusion, most used brasses for naval industry are:
• Phosphor bronze
• Aluminium bronze
• Silicon bronze
In chapter 2.4 I will give more information about the use of bronze in naval industry, giving some examples of pieces made of this metal.
2.3 Main differences between using brass and bronze
The main metal from booth alloys, as explained before, is copper, but depending on the other metals added, the properties of the material would change. In conclusion, depending on the use, different brasses or bonzes can be chosen. In the following table are resumed the main differences between booth metals.
History Due to the difficulty of getting zinc, the
production has been delayed until 18th century.
Use of bronze dates approximately about 3000BC.
Composition Mainly copper and zinc, but other metals
can be added to the alloy.
The alloy consists primarily of copper and tin as the main additive. To this base, sometimes other elements can be added.
Main properties 1. Higher malleability than zinc or
2. Low melting point (900ºC).
3.The combinations of iron, aluminium, silicon and manganese improves the anti-corrosive properties of the alloy. 4. Not hard as steel.
1. Hard but brittle material.
2. Low melting point (950ºC). It depends basically on the tin percentage of the alloy. 3. Resists especially seawater corrosion. 4. Better conductor of electricity and heat than most of steels.
Colour Most of the alloys have different shades
Uses 1. Decorative
2. Low-friction applications 3. Musical instruments
4. Anti-spark tools for flammable environments
5. Fittings for boats and ships
1. Fittings for boats and ships 2. Boats and ships propellers 3. Sea-water submerged bearings 4. For casted sculptures
5. Electrical connectors 6. Bells and cymbals
2.4 Uses of brass and bronze in naval industry
Brass and bronze are usually used in marine environments mainly due to the great performance of these metals against corrosion, as good as for their great mechanical performance. It is also used due to its golden colour and because it is very easy to get shine again after some time of use. Thanks to these properties, brass and bronze are very used for furniture and decorative objects. Some examples of this can be:
Hinges are usually fitted in doors and all other kind of furniture that have to be opened. In most cases, that hinges are made of phosphorus bronze due to their good low friction coefficient, ideal for reducing the material wear. This material is also used do to its rusting resistance against marine environment.
Figure 8. Bronze hinge. Source: www.morehandles.co.uk
b) Locks and levers for doors
As in the previous case, it is necessary to avoid the wearing of the piece do to its use. Due to this main premise, added to the corrosion resistance, it is possible to use phosphorus bronze.
Figure 9. Bronze lock. Source: www.force4.co.uk
c) Door handle
Door handles are only used for decorative purposes, so it is only necessary resistance against sea environment. Brass and bronze are good for this purpose, so depending on the colour desired (yellow or reddish), one or the other will be chosen.
15 Figure 10. Brass handle. Source: www.premierdoorhandles.co.uk
d) Wall lamps
As in door handles, it is only used for decorative purposes. It is very important that the material has good resistance against sea water in case it is placed at outdoor (it is permanently in contact with water). Any kind of brass or bronze can be used for this purpose, depending on the colour desired (yellow or reddish).
Figure 11. Bronze wall lamp. Source: www.lightiningandceilingfans.com
e) Metal parts of clocks (or any other decorative furniture)
As in wall lamps, those objects are only used for decorative purposes; in conclusion, it only necessary that the material used resists the marine environment, avoiding rusting. Any kind of brass or bronze can be used, choosing one or another only depending on the colour desired (yellow or reddish).
Due to the good performance against marine environment, and good strength properties, those metals are also used for plumbing accessories in nautical industry. Some examples are:
For all the pieces in contact with seawater it is necessary a good performance against corrosion. In conclusion, for the through-hull the most used material is the phosphor bronze.
Figure 13. Bronze through-hull. Source: www.nauticexpo.es
All the valves installed in a ship will be in contact with the seawater that goes through them. For this reason, it is very important that the valve material has a good performance against corrosion. Most used material for valves is phosphor bronze.
Figure 14. Bronze valve. Source: www.nauticaglobal.es
c) Trunk connection
For all the pieces in contact with seawater it is necessary a good performance against corrosion. In conclusion, for the trunk connection the most used materials are phosphor bronze and naval brass.
17 Those are not the only uses in the maritime world of copper alloys; it is also used for the construction of ship propellers. For small, as good as for big propellers, the most used alloy for manufacturing the screw is the aluminium bronze.
Figure 16. Small bronze propeller. Source: www.sodel.com
As commented before (see chapter 2.2.2), this alloy is composed by 5-11% of aluminium and 89-95% of copper. Normally some nickel can be added to the alloy in order to ensure better properties of the material.
The main reasons of using aluminium bronze use for propellers are: - It is very resistance to the sea water corrosion.
- It is also useful for reducing the accumulation of marine organisms
- The phenomenon of cavitation is reduced thanks to this alloy. In conclusion, even after several time of using the propeller, the surface keeps very smooth. This allows us having always a great performance, increasing the fuel efficiency.
- As there is aluminium in the alloy, the weight of the screw is reduced. This is important to reduce the bending in the propellers shaft.
- It has excellent resistance to bending, breaking and wearing.
- It needs less maintenance because of its good mechanical properties.
Chapter 3. Polishing methods.
For most industries a good final surface of the pieces is needed. To obtain this quality after manufacture the piece, it is necessary another process: the polishing. Over the years the polishing systems have improved and evolved.
The objective of all polishing systems is to transform a rough surface into a smooth one. Depending on the initial surface condition, will be needed different procedures. Thinking about the surface magnified thousand times, it is possible to see mountains and valleys of material, so the purpose of the polishing procedure is to wear down all those mountains, leaving a flat surface. In conclusion, for our eyes, before doing any treatment the surface will dissipate the light, but after the polishing process, light will not be dissipated, will be reflected, allowing the piece to shine.
In the following Figure 18. Reflection differences in a polished / not polished surface. Source: www.cdn.britannica.com it is represented the difference between a polished surface, and a rough surface. As it is possible to see, the light will not have the same performance in both cases.
Figure 18. Reflection differences in a polished / not polished surface. Source: www.cdn.britannica.com
In most cases, to complete the whole polishing process and have this final surface, are needed different steps:
1. Rough down the surface
It is the first step of the process and in those systems are used very abrasive materials. Thanks to it, we will able to remove biggest imperfections of the piece before starting the polishing process.
Rough down has also a negative part, it produces new scratches at the piece because of the abrasiveness of the material used.
This process is only necessary when there are very big imperfections (like welding strips, burs, etc.), and you want to remove them efficiently. In conclusion, it is not an obligatory step in all cases.
It is used to smooth the surface and decrease the rugosity in the whole piece. In this step is necessary to attack the metal with less abrasive materials, in order to decrease the scratches that has appeared due to the manufacturing of the piece or during the first step above described. 3. Polishing
It is the final step required. It is necessary the use of the lowest abrasive options. Depending on the polishing material, we can obtain different type of final surfaces:
- Mirror finish - Matt finish - Satin finish - Gloss finish - Etching finish
Normally in one process is not possible to cover all the steps described before. Each step can be complemented with another process on the same machine, or also with another system, to improve the final result.
21 Graphic 2. Main polishing solutions. Source: Own
Of all those systems listed before, I will describe: - Theory of the polishing system - Description of the machine - Materials needed for polishing
- Recommendations for polishing brass and bronze - Advantages and disadvantages of the method
Of all the processes described in Graphic 2, in Chapter 3 I will analyse manual polishing, disc finishing, vibratory polishing, barrel finishing and electro-polishing. Electro-mechanical polishing will be described in a separate chapter (chapter number 4) because it is the process used in the EN-34, the machine which has to be improved.
3.2 Manual polishing
3.2.1. Theory of the system
This is the simplest way for polishing but is also the most laborious of all. Basically, we have a motor connected to an abrasive wheel. Thanks to the velocity that the motor reaches and the abrasiveness of the material of the wheel, the operator can wear away manually the metal piece placing it in contact with the wheel.
In these machines the operator needs good knowledge about how to polish (pressure between the wheel and the piece, angle attack between the wheel and the piece, etc.) and all the steps needed to obtain a
methodsManual polishing Disc finishing •Wet •Dry Vibratory polishing •Wet •Dry Barrel finishing •Wet •Dry Electro-polishing Electro-mechanical polishing
good final result. Obviously, depending on their skills they will have better results. The most important thing is the material of the wheel and the polishing compound used. This will affect directly to the final result obtained.
In conclusion, thanks to the rotation of the spindle motor connected to the wheel, and the movement of the piece in different directions by the operator, there is an erosion of the piece surface.
Figure 19. Use of a manual polishing motor. Source: www.theprecisiontools.com
3.2.2. Description of the machine
The machine is set up by an electrical motor, which normally has two outputs, two spindles, where is possible to fit the different wheels.
When the machine is switched on, the motor starts running so the wheel starts the rotation. The operator can starts polishing, first placing the piece in contact with the wheel and then moving it in different orientations to polish all the parts. We can differentiate three types of machines, depending where can be placed.
It needs to be fitted in a bench with its own subjection system. It is used for smaller pieces because of its size and speed rotation (less than other kind of grinders).
23 Pedestal grinder
This model is bigger than the other because has a body that allows to the machine to be fitted directly at the floor. It is possible to use it for bigger pieces.
Figure 21. Pedestal grinder. Source: www.bigcommerce.com
Grinder fitted in a cabin.
In this case the motor is fitted inside a cabin that can be put on top of a table. It is usually used for jewellery, and this design is thought to work while the operator is seated on a chair. Thanks to an extractor system, it is possible to recover all the metal removed from the pieces (very important for precious metals).
Figure 22. Grinder used mainly in jewellery. Source: www.cdn.shopify.com
In each machine we can basically differentiate the following parts: 1) Motor.
Gives the rotational movement to the polishing wheel. The power and the rotational velocity are the main characteristics of the machine.
It is a shaft where is possible to fit the polishing wheel. Normally these machines have two spindles, so we will be able to have two kinds of wheels at the same time fitted in the machine.
Allows the machine to start running. 4) Eye protector.
It is a security part, which has to be covering the wheel while the machine is running, in order to avoid that some metal removal goes to the operator.
5) Hand support.
Depending on the machine, there is a support where the operator can rest the hand while he is doing the polishing process over the piece.
6) Abrasive wheel.
It is the part used to make the polishing. There are different types, depending on the final surface desired.
Figure 23. Differentiate parts of a bench grinder. Source: www.metalartspress.com
3.2.3. Materials used for polishing
For manual polishing it is necessary two kind of materials: abrasive wheels and polishing pastes. Abrasive wheels
They are placed in the spindle of the machine and they are used for removing the metal from the surface of the piece. Many different kinds of abrasive can be used, depending on the desired final surface.
25 The size of the wheel basically depends on the machine used (total diameter allowed to install in the machine) and the part needed to be polished (the piece will determine the width of the wheel).
Figure 24. Different examples of abrasive wheels. Source: www.taberindustries.com
Depending on the desired final surface, we normally use different wheel materials. In other words, all these abrasive wheels (described in the following lines) can be used for all kind of metals, but the result on the surface will be different (depending on the hardness of the material to polish, the results will be different).
Graphic 3. Abrasives wheels used for manual polishing. Source: Own
In the following lines I will describe the most common materials used for polishing wheels.
a) Cotton and muslin wheels
This soft material is generally used for the final part of polishing process. It is possible to classify those wheels in:
It is a soft material wheel, very used for finishing the piece after all the rough process. - Uncombed.
Cotton and muslin
Nylon and wire
Thanks to their structure, those wheels have a harder surface than the typical combed ones. Thanks to this property, they can be great for rough finishing and for removing scratches.
It is usually used to give a final high polished surface. More row stitches will give more stiffness to the whole wheel, allowing to the operator applying more pressure against the piece.
It is a very soft and flexible wheel, very common for final finishing. As it is a very soft material, is perfect for contoured edges and curves.
This kind of wheels usually live longer and have a better compound retention (in comparison with the other types described). It comes in a wide type of varieties, from aggressive abrasion as good as for giving a final polished surface.
Figure 25. Different cotton polishing wheels. Source: www.panadent.co.uk
b) Felt wheels
These wheels are made of dense and tightly compressed wool felt. They are considered of medium hardness, so are suitable for all polishing purposes. Depending on their density they can be extra hard.
Figure 26. Different sizes of felt wheels. Source: www.victoryhardware.com.sg
27 The nylon and wire assembled brushes to the wheel are usually used for cleaning, deburring and smoothing rough surfaces. Those brushes can be made also from other materials like bass or steel bristles. Depending on the material, the wheel will be good for different tasks.
Figure 27. Steel wire wheel. Source. www.amazon.com
Figure 28. Nylon wheel. Source: www.public.snapon.com
d) Abrasive wheel
Those types of wheels are made of abrasive grains joined thanks to a binder material. This wheel is also reinforced with a metallic mesh, which is useful to have pores between the grains. It is possible to have different kind of wheels, depending on some parameters:
1. Type of abrasive grain
It is possible to have two different abrasive grains; the aluminium oxide and the silicon carbide. - Aluminium oxide flap wheels
This wheel incorporates an abrasive granule of aluminium oxide. Depending on the hardness of the material needed to be processed, it can be used for deburring, polishing or to create a satin finish.
Figure 29. Aluminium oxide wheel. Source: www.amleo.com
- Silicon carbide wheels
These types of wheels are very strong so they are normally used for grinding (instead of polishing).
Figure 30. Silicon carbide wheel. Source: www.exportersindia.com
2. Grain size
It is the grain dimensions and it is possible to divide the grain sizes in: - Thin grains.
These grains are used to obtain different smooth surfaces in hard and breakable materials. - Heavy grains
These grains are used in soft and fibrous materials for removing quickly material from the surface. 3. Hardness grade
It is the capacity of the binder material to maintain the abrasive grains together with the wheel. We can divide the hardness between:
If it is soft, the binder is not able to maintain together all the grains, so those grains will detach. This can be good because the wheel will sharpen automatically.
If it is very hard, the grains are joined very tightly so these wheels will have a longer live. 4. Structure
29 The structure represents the distance between the grains in a wheel. Depending on the material of the piece needed to be polished, the material speed elimination, the precision and the final surface required, we will choose between different kind of structures.
5. Binder material
It is the material used to join the abrasive grains. The type of binder material depends on the working speed of the wheel and the required final surface. Some binder materials are:
o Synthetic resins /Bakelite
o Oxychloride o Rubber o Reinforced rubber o Silicate o Ceramic Polishing pastes
In these machines is not enough with the correct type of polishing wheel, it is also necessary the use of a polishing paste to have the desired final surface. There are different kinds of polishing pastes, depending on the material needed to be polished. The paste is added to the abrasive wheels in order to facilitate the metal removing.
Figure 31. Different examples of polishing pastes. Source: www.divinebrothers.com
These pastes are made by a mixture of polish, wax and metallic rust. The buffing compounds are mainly used with the polishing or buffing wheels (described before), and depending on the material needed to be polished we will choose one or another kind of compound.
Those materials help the operator doing the polishing process faster. Some of them are rougher, so are useful to remove the material faster (to remove all the scratches and imperfections), and others are softer, so are designed to obtain a beautiful finished surface.
Depending on the material and the desired finishing (mirror, satin, gloss, etc.), it is necessary a different type of paste. Normally, the colour of the paste determines the properties, so it is possible to classify those consumables as shown in the graphic below.
Graphic 4. Compounds used for manual polishing. Source: Own
Now, once the different kind of polishing pastes are named, I will describe the different compounds used, depending on its colour.
1. Black compound.
This compound is made of emery minerals. It allows the removing of scratches, small pitting, rough surfaces, etc. It is very useful when there are a lot of imperfections, because you can save time of the polishing process.
Figure 32. Black compound for manual polishing. Source: www.picclick.co.uk
2. Brown Tripoli
This compound is useful for two purposes: grinding and polishing. The compound can easily remove scratches while is leaving a smooth finish. For example, it is a good solution for soft materials as brass, copper or aluminium.
Figure 33. Brown compound for manual polishing. Source: www.goshineon.com
sBlack compound Brown Tripoli White rouge Red rouge Green rouge Tan compound Orange-glow compound Blue magic
31 3. White rouge
It is great for hard metals like chrome or nickel-plated things. It gives good shine to the surface of those kind of alloys.
Figure 34. White rouge compound for manual polishing. Source: www.jewelquestmarketing.com
4. Red rouge (or jeweller’s rouge)
It is ideal for high quality finishing in gold, silver and other precious metals. This consumable gives to the metal a true colour, at the same time that they will shine as like new.
Figure 35. Red rouge compound for manual polishing. Source: www.silversupplies.com
5. Green rouge
It is designed to provide a high shinny finish on all type of materials (soft and hard). Despite is good for all materials, has better performance with chrome, stainless steel and platinum.
Figure 36. Green rouge compound for manual polishing. Source: www.goshineon.com
6. Tan compound
It is known for its fast grinding characteristics, so is an ideal pre-polishing compound for removing light scratches. It can give a good performance in gold and silver if it is used together with buffing wheels.
Figure 37. Tan compound for manual polishing. Source: www.riogrande.com
7. Orange-glow compound
This is normally used for platinum, white/yellow gold and stainless steel to give a very shiny surface.
Figure 38. Orange-glow compound for manual polishing. Source: www.es-dental.keystoneindustries.com
8. Blue magic
It is designed to give a high-quality shine to the platinum jewellery, as well as for other type of precious metals.
Figure 39. Blue magic compound for manual polishing. Source: www.goshineon.com
3.2.4. Parameters recommended for polishing brass and bronze
In next paragraphs I will give some recommendations for polishing brass or bronze from casting. In this polishing system are needed different steps to get the final desired surface, so I will give the best parameters to get shiny results. It is advisable to do all those steps with a motor at 3000 rpm.
- Rough down the surface
It is advisable to use a silicon carbide wheel in order to remove all big imperfections that the piece have after casting. Depending on the initial surface, we will use one grain size or another.
Previous step produces new scratches in the surface that must be removed, so before giving the final polishing surface to the piece, it is advisable to use the combination of an uncombed wheel and brown tripoli compound.
For brass and bronze, to get the desired shine and polished final surface, it is recommended to use an unstitched wheel with green rouge compound.
3.2.5. Advantages and disadvantages of the system
After seeing all this information about this polishing system, I can conclude that there are some advantages and disadvantages.
• Simple polishing machines.
• Machines are not expensive, so it is affordable for most companies.
• Useful for easy pieces. If they have a lot of flat surfaces it is a good solution. DISADVANTAGES
• Polishing needs three different steps in order to have a good final surface.
• Many different types of abrasive wheels and polishing pastes are needed, depending on the material and the final finish required.
• The final result depends exclusively on the polishing experience of the operator.
• For large productions you need a lot of operators, which means a lot of salaries.
• Depending on the shape of the piece, will be necessary more or less polishing time. For difficult pieces it will be necessary to use more time in order to have a good finishing.
• As it is a manual polishing, it is difficult to respect the geometry of the piece. In other words; for critical shapes, it is not a very good system.
• As there is mainly man interaction, it is provable that some pieces do not have the final desired result, so they will be rejected.
After seeing all the advantages and disadvantages from manual polishing, I can conclude that manual polishing is interesting for those small brass and bronze pieces which have opened and flat surfaces, also as where respecting the initial geometry of the piece is not very important. Some pieces examples are:
• Door handle
• Clock’s and decorative parts
• Small ship’s screws
Big ship propellers cannot be done with any machine described before due its dimensions, so the most common option is doing all the polishing process with an angular grinding machine. As this machine is easily transportable, it gives freedom to the operator, allowing him to move without any dimension restriction. This method is also very useful because can also be used when the propeller is inside the water (for maintenance tasks).
Figure 40. Polishing a bronze propeller inside the water with an angular grinding machine. Source: www.dynamicdivers.gr
For each polishing method I will give a punctuation depending on its effectiveness and limitations in different parameters. After all methods are described, it will be possible to compare all of them in order to see the better one for naval industry.
The punctuation system will be as follows:
+ + Very convenient + Convenient
- Not convenient
- - Nothing at all convenient
For manual polishing, the punctuation is described in the below table:
Polishing method Cost of machine Consumables cost Polishing time Polishing quality Automatic process Number of pieces / process Use in big pieces Use in small pieces Noise Manual polishing + + + - - - - - - + + - -
35 3.3 Disc finishing machine
3.3.1. Theory of the system
Disc polishing machine works using a drum with a (rotary) disc placed at the bottom. The rotation of the disc creates a centrifugal force, allowing the pieces and media to move upward while there is also a rotating movement. The pieces and the media have different weight, so the centrifugal force is different for both.
This movement creates a rolling action between pieces and media, causing erosion of these two components, but not of the drum, because it is covered with a polyurethane liner that can stand up a repeated friction.
Figure 41. Movement of the pieces inside the disc finishing machine. Source: www.makromakine.com.tr
For a good final surface of the pieces, the final result can depend on many different parameters:
• Quality, shape and size of the abrasive media
• Type, capacity and design of the machine